The Fundamental Principles of Composite Material Stiffness Predictions. David Richardson


 Brice Bailey
 3 years ago
 Views:
Transcription
1 The Fundamental Principles of Composite Material Stiffness Predictions David Richardson
2 Contents Description of example material for analysis Prediction of Stiffness using Rule of Mixtures (ROM) ROM with Efficiency Factor Hart Smith 10% rule Classical Laminate Analysis Simplified approach Overview of misconceptions in material property comparison between isotropic materials and composites
3 Lamina Axis Notation Diagram taken from Harris (1999)
4 Example Material for Analysis M21/35%/UD268/T700 A common Aerospace unidirectional prepreg material called HexPly M21 from Hexcel E f = 235 GPa ρ f = 1.78 g/cm3 E m = 3.5 GPa ρ m = 1.28 g/cm3 W r = 35% (composite resin weight fraction) Layup = (0/0/0/+45/45/0/0/0)
5 Stage 1 Convert fibre weight fraction of composite to fibre volume fraction Fibre weight fraction used by material suppliers Fibre volume fraction needed for calculations
6 Fibre Volume Fraction Fibre mass fraction of M21 = 65% (0.65) Data sheet says material is 35% resin by weight, therefore 65% fibre by weight Calculation of fibre volume fraction The resulting volume fraction is 57.2% V f W f f W f f W m m
7 Methods of Stiffness Prediction Rule of Mixtures (with efficiency factor) HartSmith 10% Rule Used in aerospace industry as a quick method of estimating stiffness Empirical Formulae Based solely on test data Classical Laminate Analysis LAP software
8 Rule of Mixtures A composite is a mixture or combination of two (or more) materials The Rule of Mixtures formula can be used to calculate / predict Young s Modulus (E) Density Poisson s ratio Strength (UTS) very optimistic prediction 50% usually measured in test Strength very difficult to predict numerous reasons
9 Rule of Mixtures for Stiffness Rule of Mixtures for Young s Modulus Assumes unidirectional fibres Predicts Young s Modulus in fibre direction only E c = E f V f + E m V m Ec = E c = 136 GPa
10 Rule of Mixtures: Efficiency Factor The Efficiency Factor or Krenchel factor can be used to predict the effect of fibre orientation on stiffness This is a term that is used to factor the Rule of Mixtures formula according to the fibre angle See following slide
11 Reinforcing Efficiency a n = proportion of total fibre content θ = angle of fibres η θ = composite efficiency factor (Krenchel)
12 Efficiency (Krenchel) Factor Diagram taken from Harris (1999)
13 Prediction of E for Example Ply E f = 235 GPa E m = 3.5 GPa V f = E(θ) = (Cos 4 θ ) + ( ) Predicted modulus versus angle plotted on following slide
14 Tensile Modulus (GPa) Prediction of Tensile Modulus (Efficiency Factor) Angle (degrees)
15 Efficiency Factor for Laminate Layup = (0/0/0/+45/45/0/0/0) η = Cos 4 θ 0 = η = 1 45 = η = = η = 0 Laminate in Xdirection (6/8 1) + (2/8 0.25) ( ) Laminate in Ydirection (6/8 0) + (2/8 0.25) ( )
16 Prediction of E for Example Ply E f = 235 GPa E m = 3.5 GPa V f = E x = ( ) + ( ) E x = = GPa E y = ( ) + ( ) E y = = 9.9 GPa
17 TenPercent Rule HartSmith 1993 Each 45 or 90 ply is considered to contribute one tenth of the strength or stiffness of a 0 ply to the overall performance of the laminate Rapid and reasonably accurate estimate Used in Aerospace industry where standard layup [0/±45/90] is usually used E x = E 11. ( % plies at 0 ) σ x = σ 11. ( % plies at 0 ) G xy = E 11. ( % plies at ± 45 )
18 Tensile Modulus (GPa) Prediction of Tensile Modulus ROM 80 HartSmith Angle (degrees)
19 Calculation of E 11 for Ply Using Rule of Mixtures E 11 = E f V f + E m V m E 11 = E 11 = 136 GPa Layup = (0/0/0/+45/45/0/0/0) 6/8 = 75% of plies in zero degree direction
20 TenPercent Rule E x = E 11 ( % plies at 0 ) E x = 136 (0.1 + ( )) E x = 136 (0.775) E x = GPa E y = E 11 ( % plies at 0 ) E y = 136 (0.1 + (0.9 0)) E y = 136 (0.1) E y = 13.6 GPa
21 Classical Laminate Analysis 4 elastic constants are needed to characterise the inplane macroscopic elastic properties of a ply E 11 = Longitudinal Stiffness E 22 = Transverse Stiffness ν 12 = Major Poisson s Ratio G 12 = InPlane Shear Modulus
22 Elastic Constant Equations E 11 = Longitudinal Stiffness (Rule of Mixtures Formulae) E 22 = Transverse Stiffness (Inverse Rule of Mixtures Formulae (Reuss Model)) ν 12 = Major Poisson s Ratio (Rule of Mixtures for Poisson s Ratio) G 12 = InPlane Shear Modulus (Inverse Rule of Mixtures for Shear)
23 Calculation of E 11 for Ply Using Rule of Mixtures E 11 = E f V f + E m V m E 11 = E 11 = 136 GPa
24 Calculation of E 22 for Ply Using Inverse Rule of Mixtures Formulae (Reuss Model) E 22 = 8 GPa
25 Calculate Poisson s Ratio (ν 12 ) for Ply Using Rule of Mixtures formula However, we do not know Poisson s ratio for carbon fibre Poisson s ratio for epoxy matrix We would need to find these for accurate prediction We will assume a Poisson s Ratio (ν) of 0.3
26 Calculate Shear Modulus (G 12 ) of Ply Using Inverse Rule of Mixtures formula G for carbon fibre = 52 GPa (from test) G for epoxy = 2.26 GPa (from test) Both calculated using standard shear modulus formula G = E/(2(1+ν)) G 12 for composite = 5 GPa
27 Resulting Properties of Ply E 11 = 136 GPa E 22 = 8 GPa ν 12 = 0.3 G 12 = 5 GPa
28 Matrix Representation 4 material elastic properties are needed to charaterise the inplane behaviour of the linear elastic orthotropic ply We conveniently define these in terms of measured engineering constants (as above) These are usually expressed in matrix form due to large equations produced and subsequent manipulations required The stiffness matrix [Q] The compliance matrix [S] (inverse of stiffness)
29 Offaxis Orientation & Analysis The stiffness matrix is defined in terms of principal material directions, E 11, E 22 However, we need to analyse or predict the material properties in other directions As it is unlikely to be loaded only in principal direction We use stress transformation equations for this Related to Mohr s stress circle The transformation equations are written in matrix form They have nothing to do with the material properties, they are merely a rotation of stresses.
30 Single Ply [6 x 6] stiffness matrix [C] or [6 x 6] compliance matrix [S] Often reduced stiffness matrix [Q] for orthotropic laminates [3 x 3] Orthotropic = 3 mutually orthogonal planes of symetry 4 elastic constants characterise the behaviour of the laminate E1, E2, υ12, G12
31 Stiffness & Compliance Martricies Stiffness Matrix [Q] Calculates laminate stresses from laminate strains Compliance Matrix [S] Calculates laminate strains from laminate stresses (inverse of compliance)
32 Transformation Matrix The stress transformation equation that relates known stresses in the z, y coordinate system to stresses in the L, T coordinate system. These are related to the transformation performed using Mohr s stress circle.
33 Transformed Stiffness Components
34 Transformed Compliance Components
35 Individual Compliance & Stiffness terms
36 CLA Derived Formula Formula from Engineering Design with Polymers and Composites, J.C.Gerdeen et al. Suitable for calculating Young s Modulus of a unidirectional ply at different angles.
37 Example Material (θ = 0 ) E 11 = 136 GPa, E 22 = 8 GPa ν 12 = 0.3, G 12 = 5 GPa 1/E x = 1/ E x for 0 fibres = 136 GPa
38 Example Material (θ = 45 ) E 11 = 136 GPa, E 22 = 8 GPa ν 12 = 0.3, G 12 = 5 GPa 1/E x = 0.25/ /8 + ( 1/50.6/136 ) /E x = 0.25/ /8 + ( 1/50.6/136 ) 0.25 E x for 45 fibres = 12.2 GPa
39 Example Material (θ = 90 ) E 11 = 136 GPa, E 22 = 8 GPa ν 12 = 0.3, G 12 = 5 GPa 1/E x = 0 + 1/8 + 0 E x for 90 fibres = 8 GPa
40 Properties of Laminate CFRE (0/0/0/+45/45/0/0/0) 0 = 136 GPa 45 = 12.2GPa 90 = 8 GPa Laminate in Xdirection (6/8 136) + (2/8 12.2) = 105 GPa Laminate in Ydirection (6/8 8) + (2/8 12.2) = 9 GPa Note: This simplified calculation ignores the effect of coupling between extension and shear
41 Classical Laminate Analysis The simplified laminate analysis approach taken ignores the effect of coupling between extension and shear Classical Laminate Analysis takes full account of this effect However, this is too long and complex for hand calculations Therefore build a spreadsheet or use software such as LAP (Laminate Analysis Programme)
42 Summary of Results For HexPly M21 Prepreg with (0/0/0/+45/45/0/0/0) layup ROM & Efficiency factor HartSmith 10% Rule ROM of CLA rotation formula Classical Laminate Analysis LAP E x E y
43 Tensile Modulus (GPa) Prediction of Tensile Modulus CLA ROM 80 HartSmith Angle (degrees)
44 Procedure for Structural Analysis Classical Laminate Analysis to provide Relationship between inplane load and strain Relationship between out of plane bending moments and curvatures Plate properties from the A, B and D matrices Then analysis is equivalent to classical analysis of anisotropic materials FE analysis Standard formulas to check stiffness
45 Material Property Comparison Young s Modulus of materials Isotropic Materials Aluminium = 70 GPa Steel = 210 GPa Polymers = 3 GPa Fibres Carbon = 240 GPa common high strength T700 fibre Glass = 70 GPa
46 Care with Property Comparison E for Aluminium = 70 GPa E for Glass fibre = 70 GPa However. 50% fibre volume fraction E now 35 GPa in xdirection E in ydirection = matrix = 3 GPa 0/90 woven fabric 50% of material in each direction E now 17.5 GPa in x and y direction E at 45 = 9 GPa Glass reinforced polymer composite now has a low stiffness compared to Aluminium!
47 Stress (MPa) 2000 UD CFRE 50% Fv (E = 120 GPa) CFRE is elastic until ultimate failure (no plasticity) /90 CFRE 50% Fv (E = 60 GPa) Elasticity until failure (no plasticity) 1000 QuasiIsotropic CFRE 50% Fv (E = 45 GPa) Elasticity until failure (no plasticity) 500 Yield Point  Elastic to here Aluminium (E = 70 GPa) Elastic until yield point, then followed by large range of plasticity. Design to yield  therefore beneficial plasticity safety zone. Strain
48 References & Bibliography Engineering Design with Polymers and Composites J.C.Gerdeen, H.W.Lord & R.A.L.Rorrer Taylor and Francis, 2006 Engineering Composite Materials Bryan Harris, Bath University Composite Materials  UWE Elearning resource David Richardson, John Burns & Aerocomp Ltd.
49 Contact Details Dr David Richardson Room 1N22 Faculty of Engineering and Technology University of the West of England Frenchay Campus Coldharbour Lane Bristol BS16 1QY Tel:
Composite Design Fundamentals. David Richardson
Composite Design Fundamentals David Richardson Contents A review of the fundamental characteristics of composites Stiffness and Strength Anisotropic Role of fibre, matrix and interface Composite failure
More informationProduct Data. HexPly 8552 Epoxy matrix (180 C/356 F curing matrix)
HexPly 8552 Epoxy matrix (180 C/356 F curing matrix) Product Data Description HexPly 8552 is a high performance tough epoxy matrix for use in primary aerospace structures. It exhibits good impact resistance
More informationIntroduction to Aerospace Engineering
Introduction to Aerospace Engineering Lecture slides Challenge the future 1 Material types Metals, polymers, ceramics, composites Faculty of Aerospace Engineering 6122011 Delft University of Technology
More informationExperiment: Fiber Reinforced Composite Materials
Experiment: Fiber Reinforced Composite Materials Objective To investigate the strength and stiffness characteristics of laminated composite materials as a function of fiber orientation. Abstract Composites
More informationCARBON/DYNEEMA INTRALAMINAR HYBRIDS: NEW STRATEGY TO INCREASE IMPACT RESISTANCE OR DECREASE MASS OF CARBON FIBER COMPOSITES
26 TH INTERNATIONAL CONGRESS OF THE AERONAUTICAL SCIENCES CARBON/DYNEEMA INTRALAMINAR HYBRIDS: NEW STRATEGY TO INCREASE IMPACT RESISTANCE OR DECREASE MASS OF CARBON FIBER COMPOSITES J. G. H. Bouwmeester*,
More informationDesign of Carbon Composite Driveshaft for Ultralight Aircraft Propulsion System R. Poul, P. Růžička,. D. Hanus, K. Blahouš
Design of Carbon Composite Driveshaft for Ultralight Aircraft Propulsion System R. Poul, P. Růžička,. D. Hanus, K. Blahouš This paper deals with the design of the carbon fibre composite driveshaft. This
More informationTECHNICAL DATA SHEET
EPOXY  NG1001 Formulated Resin System for Prepreg Process General information Description: TECHNICAL DATA SHEET EPOXY  NG1001 is a formulated epoxy based resin system for hot melt prepreg and pressure
More informationINVESTIGATION OF VISCOELASTICITY AND CURE SHRINKAGE IN AN EPOXY RESIN DURING PROCESSING
TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS INVESTIGATION OF VISCOELASTICITY AND CURE SHRINKAGE IN AN EPOXY RESIN DURING PROCESSING T. Shimizu *, H. Koinuma, K. Nagai Mitsubishi Heavy Industries,
More informationTHE COMPOSITE DISC  A NEW JOINT FOR HIGH POWER DRIVESHAFTS
THE COMPOSITE DISC  A NEW JOINT FOR HIGH POWER DRIVESHAFTS Dr Andrew Pollard Principal Engineer GKN Technology UK INTRODUCTION There is a wide choice of flexible couplings for power transmission applications,
More informationCommon Layup Terms and Conditions
MidPlane: Centerline of the layup. Plane forming the midline of the laminate. Symmetry: A laminate is symmetric when the plies above the midplane are a mirror image of those below the midplane. Symmetrical
More informationLap Fillet Weld Calculations and FEA Techniques
Lap Fillet Weld Calculations and FEA Techniques By: MS.ME Ahmad A. Abbas Sr. Analysis Engineer Ahmad.Abbas@AdvancedCAE.com www.advancedcae.com Sunday, July 11, 2010 Advanced CAE All contents Copyright
More informationMatrix system with enhanced mechanical performance: new infusion system for wind energy applications enables lighter, longer, lower cost rotor blades
White Paper Matrix system with enhanced mechanical performance: new infusion system for wind energy applications enables lighter, longer, lower cost rotor blades Malte Wichmann Momentive Specialty Chemicals
More information(Seattle is home of Boeing Jets)
Dr. Faeq M. Shaikh Seattle, Washington, USA (Seattle is home of Boeing Jets) 1 Pre Requisites for Today s Seminar Basic understanding of Finite Element Analysis Working Knowledge of Laminate Plate Theory
More informationUse of Strain Gauge Rosette to Investigate Stress concentration in Isotropic and Orthotropic Plate with Circular Hole
Use of Strain Gauge Rosette to Investigate Stress concentration in Isotropic and Orthotropic Plate with Circular Hole Mr.V.G.Aradhye 1, Prof.S.S.Kulkarni 2 1 PG Scholar, Mechanical department, SKN Sinhgad
More informationA NOVEL STRENGTH MODEL FOR UNIDIRECTIONAL FIBRE REINFORCED COMPOSITES WITH REALISTIC FIBRE PACKINGS
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS A NOVEL STRENGTH MODEL FOR UNIDIRECTIONAL FIBRE REINFORCED COMPOSITES WITH REALISTIC FIBRE PACKINGS Y. Swolfs 1, L. Gorbatikh 1, I. Verpoest*
More informationThe elements used in commercial codes can be classified in two basic categories:
CHAPTER 3 Truss Element 3.1 Introduction The single most important concept in understanding FEA, is the basic understanding of various finite elements that we employ in an analysis. Elements are used for
More information1 of 79 Erik Eberhardt UBC Geological Engineering EOSC 433
Stress & Strain: A review xx yz zz zx zy xy xz yx yy xx yy zz 1 of 79 Erik Eberhardt UBC Geological Engineering EOSC 433 Disclaimer before beginning your problem assignment: Pick up and compare any set
More informationMechanical Properties  Stresses & Strains
Mechanical Properties  Stresses & Strains Types of Deformation : Elasic Plastic Anelastic Elastic deformation is defined as instantaneous recoverable deformation Hooke's law : For tensile loading, σ =
More informationCOMPARISON BETWEEN GLASS AND FLAX NONCRIMP STITCHED FABRICS
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS COMPARISON BETWEEN GLASS AND FLAX NONCRIMP STITCHED FABRICS L. Bizet 1 *, S. Guéret 1, C. Re 1, P. Ouagne 2 1 Laboratoire Ondes et Milieux Complexes,
More informationUnit 6 Plane Stress and Plane Strain
Unit 6 Plane Stress and Plane Strain Readings: T & G 8, 9, 10, 11, 12, 14, 15, 16 Paul A. Lagace, Ph.D. Professor of Aeronautics & Astronautics and Engineering Systems There are many structural configurations
More informationMechanical Characterization of Stretch Broken Carbon Fiber Materials IM7 Fiber in 8552 Resin
Mechanical Characterization of Stretch Broken Carbon Fiber Materials IM7 Fiber in 8552 Resin Guenther Jacobsen Hexcel Corporation 6700 W. 5400 S. Salt Lake City, UT 84118 ABSTRACT Interest in aligned discontinuous
More informationExperimental validation of the 3D numerical model for an adaptive laminar wing with flexible extrados
18 th International Conference of Adaptive Structures and Technologies October 3 rd, 4 th, 5 th, 2007 Ottawa, Ontario, Canada Experimental validation of the 3D numerical model for an adaptive laminar wing
More informationMETU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING
METU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING Met E 206 MATERIALS LABORATORY EXPERIMENT 1 Prof. Dr. Rıza GÜRBÜZ Res. Assist. Gül ÇEVİK (Room: B306) INTRODUCTION TENSION TEST Mechanical testing
More informationLOW VELOCITY IMPACT ANALYSIS OF LAMINATED FRP COMPOSITES
LOW VELOCITY IMPACT ANALYSIS OF LAMINATED FRP COMPOSITES B. KRANTHI KUMAR 1 M.Tech student, Department of Mechanical Engineering, Godavari Institute of Engineering and Technology, Rajahmundry, Andhrapradesh,
More informationStress Strain Relationships
Stress Strain Relationships Tensile Testing One basic ingredient in the study of the mechanics of deformable bodies is the resistive properties of materials. These properties relate the stresses to the
More informationMaterial Optimization and Weight Reduction of Drive Shaft Using Composite Material
IOSR Journal of Mechanical and Civil Engineering (IOSRJMCE) eissn: 22781684,pISSN: 2320334X, Volume 10, Issue 1 (Nov.  Dec. 2013), PP 3946 Material Optimization and Weight Reduction of Drive Shaft
More informationBalancing Manufacturability and Optimal Structural Performance for Laminate Composites through a Genetic Algorithm
Balancing Manufacturability and Optimal Structural Performance for Laminate Composites through a Genetic Algorithm Mike Stephens Senior Composites Stress Engineer, Airbus UK Composite Research, Golf Course
More informationAnalysis of Stresses and Strains
Chapter 7 Analysis of Stresses and Strains 7.1 Introduction axial load = P / A torsional load in circular shaft = T / I p bending moment and shear force in beam = M y / I = V Q / I b in this chapter, we
More informationCertification of Discontinuous Composite Material Forms for Aircraft Structures
Certification of Discontinuous Composite Material Forms for Aircraft Structures Paolo Feraboli (UWAA), Mark Tuttle (UW), Larry Ilcewicz (FAA), Bill Avery (Boeing), Bruno Boursier, Dave Barr (Hexcel) JAMS
More informationRobust repair methods of primary structures in composite
Department of Management and Engineering, IEI LIUIEITEKG13/42 SE Robust repair methods of primary structures in composite Metal Composite Mattias Gungner Marcus Ramström Bachelor thesis in Solid Mechanics
More informationChapter 5 Bridge Deck Slabs. Bridge Engineering 1
Chapter 5 Bridge Deck Slabs Bridge Engineering 1 Basic types of bridge decks Insitu reinforced concrete deck (most common type) Precast concrete deck (minimize the use of local labor) Open steel grid
More informationThey may be based on a number of simplifying assumptions, and their use in design should tempered with extreme caution!
'Rules o Mixtures' are atheatical expressions which give soe property o the coposite in ters o the properties, quantity and arrangeent o its constituents. They ay be based on a nuber o sipliying assuptions,
More informationStress Relaxation Study of Paper and Plastic Film based Packaging Material
Master's Degree Thesis ISRN: BTHAMTEX2009/D02SE Stress Relaxation Study of Paper and Plastic Film based Packaging Material Rajdip Roy Lu Qi Department of Mechanical Engineering Blekinge Institute
More informationFatigue. Figure 41 Typical Comparison of Metal and Composite Fatigue Damage [Salkind, Fatigue of Composites]
Chapter Four PERFORMANCE Fatigue A fundamental problem concerning the engineering uses of fiber reinforced plastics (FRP) is the determination of their resistance to combined states of cyclic stress. [41]
More informationCYCOM 2040 EPOXY PREPREG
DESCRIPTION CYCOM 2040 is a very tough modified epoxy resin system with exceptional high temperature performance. It is suitable for highly stressed components exposed to elevated temperature environments
More informationFinite Element Formulation for Plates  Handout 3 
Finite Element Formulation for Plates  Handout 3  Dr Fehmi Cirak (fc286@) Completed Version Definitions A plate is a three dimensional solid body with one of the plate dimensions much smaller than the
More informationHexPly Prepreg Technology
HexPly Prepreg Technology Prepregs are specially formulated resin matrix systems that are reinforced with manmade fibres such as carbon, glass and aramid. Hexcel has its own inhouse supply of carbon
More informationDesign of a carbon fibre rim for a fuel efficient competition vehicle
FACULTY OF ENGINEERING AND SUSTAINABLE DEVELOPMENT Department of Industrial Development, IT and Land Management Design of a carbon fibre rim for a fuel efficient competition vehicle Pau Gomà Golanó 2014
More information3 Concepts of Stress Analysis
3 Concepts of Stress Analysis 3.1 Introduction Here the concepts of stress analysis will be stated in a finite element context. That means that the primary unknown will be the (generalized) displacements.
More informationUNIVERSITY OF CALIFORNIA, SAN DIEGO
UNIVERSITY OF CALIFORNIA, SAN DIEGO Structural Characterization of Concrete Filled Fiber Reinforced Shells A dissertation submitted in partial satisfaction of the requirements for the degree Doctor of
More informationMULTIPREG E644 Low Temperature Curing Toughened Epoxy Component Prepreg
E644 is a toughened epoxy resin system for low temperature cures, preimpregnated into high performance fibers such as carbon, glass & aramid. Designed for the production of composite structures in the
More informationTorsion Tests. Subjects of interest
Chapter 10 Torsion Tests Subjects of interest Introduction/Objectives Mechanical properties in torsion Torsional stresses for large plastic strains Type of torsion failures Torsion test vs.tension test
More informationInvestigation of a Macromechanical Approach to Analyzing TriaxiallyBraided Polymer Composites
NASA/TM 2010216371 AIAA 2010 2522 Investigation of a Macromechanical Approach to Analyzing TriaxiallyBraided Polymer Composites Robert K. Goldberg Glenn Research Center, Cleveland, Ohio Brina J. Blinzler
More informationCarbon Fiber Composites Low Cost Materials & Manufacturing Options
Carbon Fiber Composites Low Cost Materials & Manufacturing Options George Husman Zoltek Companies, Inc. September 13, 2012 1 Carbon Fiber Markets All China Hexcel Formosa SGL Cytec AKSA Others 2011 Estimated
More informationMASTER'S THESIS. Potential of DSP Method for Strain Distribution Analysis on Damaged Laminates
MASTER'S THESIS 2007:186 CIV Potential of DSP Method for Strain Distribution Analysis on Damaged Laminates Guillaume Dufaix Luleå University of Technology MSc Programmes in Engineering Mechanical Engineering
More informationCHARACTERIZATION OF HIGH PRESSURE RTM PROCESSES FOR MANUFACTURING OF HIGH PERFORMANCE COMPOSITES
CHARACTERIZATION OF HIGH PRESSURE RTM PROCESSES FOR MANUFACTURING OF HIGH PERFORMANCE COMPOSITES R. Chaudhari 1*, M. Karcher 1, P. Elsner 1, F. Henning 1 1 Fraunhofer Institute for Chemical Technology,
More informationUnit 48: Structural Behaviour and Detailing for Construction. Chapter 13. Reinforced Concrete Beams
Chapter 13 Reinforced Concrete Beams Concrete is a material strong in its resistance to compression, but very weak indeed in tension. good concrete will safely take a stress upwards of 7 N/mm 2 in compression,
More informationLösungen Übung Verformung
Lösungen Übung Verformung 1. (a) What is the meaning of T G? (b) To which materials does it apply? (c) What effect does it have on the toughness and on the stress strain diagram? 2. Name the four main
More informationPredictive Modeling of Composite Materials & Structures: StateoftheArt Solutions and Future Challenges.
Predictive Modeling of Composite Materials & Structures: StateoftheArt Solutions and Future Challenges. Roger A. Assaker Roger.Assaker@eXstream.com www.exstream.com Short Abstract Computer Aided Engineering
More informationINVESTIGATION OF MECHANICAL PROPERTIES OF POLYESTER REINFORCED WITH HEMP FIBRE (LONG FIBRES AND MAT) FOR PATELLAR IMPLANT APPLICATION
International Journal of Mechanical Engineering and Technology (IJMET) Volume 7, Issue 1, JanFeb 2016, pp. 154163, Article ID: IJMET_07_01_016 Available online at http://www.iaeme.com/ijmet/issues.asp?jtype=ijmet&vtype=7&itype=1
More informationCourse in. Nonlinear FEM
Course in Introduction Outline Lecture 1 Introduction Lecture 2 Geometric nonlinearity Lecture 3 Material nonlinearity Lecture 4 Material nonlinearity continued Lecture 5 Geometric nonlinearity revisited
More informationBending, Forming and Flexing Printed Circuits
Bending, Forming and Flexing Printed Circuits John Coonrod Rogers Corporation Introduction: In the printed circuit board industry there are generally two main types of circuit boards; there are rigid printed
More informationPEKK Thermoplastic Polymer
T E C H N I C A L D A T A S H E E T PEKK THERMOPLASTIC POLYMER PEKK Thermoplastic Polymer DESCRIPTION Cytec Engineered Materials PEKK composites consist of a matrix of poly(etherketoneketone) polymer with
More informationMechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied
Mechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied Stress and strain fracture or engineering point of view: allows to predict the
More informationDesign Analysis and Review of Stresses at a Point
Design Analysis and Review of Stresses at a Point Need for Design Analysis: To verify the design for safety of the structure and the users. To understand the results obtained in FEA, it is necessary to
More informationOverview of Recent Developments in 3D Structures
Overview of Recent Developments in 3D Structures Michael McClain, Senior R&T Engineer Organic Matrix Composites Jonathan Goering Divisional Chief Technology Officer Albany Engineered Composites 112 Airport
More informationComposite Materials. Mary P. Shafer. Fabric Development, Inc. Quakertown, PA 18951
Composite Materials Mary P. Shafer Fabric Development, Inc. Quakertown, PA 18951 Composite Material Two inherently different materials that when combined together produce a material with properties that
More informationα = u v. In other words, Orthogonal Projection
Orthogonal Projection Given any nonzero vector v, it is possible to decompose an arbitrary vector u into a component that points in the direction of v and one that points in a direction orthogonal to v
More informationMECHANICS OF SOLIDS  BEAMS TUTORIAL 1 STRESSES IN BEAMS DUE TO BENDING. On completion of this tutorial you should be able to do the following.
MECHANICS OF SOLIDS  BEAMS TUTOIAL 1 STESSES IN BEAMS DUE TO BENDING This is the first tutorial on bending of beams designed for anyone wishing to study it at a fairly advanced level. You should judge
More informationFree vibration of CLT plates
Rakenteiden Mekaniikka (Journal of Structural Mechanics) Vol. 47, No 1, 2014, pp. 1733 Free vibration of CLT plates JussiPekka Matilainen 1 and Jari Puttonen Summary. This article discusses the ability
More information3D Stress Components. From equilibrium principles: τ xy = τ yx, τ xz = τ zx, τ zy = τ yz. Normal Stresses. Shear Stresses
3D Stress Components From equilibrium principles:, z z, z z The most general state of stress at a point ma be represented b 6 components Normal Stresses Shear Stresses Normal stress () : the subscript
More informationThe atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
More informationStructural Integrity Analysis
Structural Integrity Analysis 1. STRESS CONCENTRATION Igor Kokcharov 1.1 STRESSES AND CONCENTRATORS 1.1.1 Stress An applied external force F causes inner forces in the carrying structure. Inner forces
More information3D PRINTING OF CONTINUOUS FIBER REINFORCED PLASTIC
3D PRINTING OF CONTINUOUS FIBER REINFORCED PLASTIC Masaki NAMIKI 1, Masahito UEDA 1, Akira TODOROKI 2 Yoshiyasu HIRANO 3, Ryosuke MATSUZAKI 4 1 Nihon University, 1814 Kandasurugadai, Chiyoda, Tokyo,
More informationCOMPUTATIONAL ENGINEERING OF FINITE ELEMENT MODELLING FOR AUTOMOTIVE APPLICATION USING ABAQUS
International Journal of Advanced Research in Engineering and Technology (IJARET) Volume 7, Issue 2, MarchApril 2016, pp. 30 52, Article ID: IJARET_07_02_004 Available online at http://www.iaeme.com/ijaret/issues.asp?jtype=ijaret&vtype=7&itype=2
More informationB.TECH. (AEROSPACE ENGINEERING) PROGRAMME (BTAE) TermEnd Examination December, 2011 BAS010 : MACHINE DESIGN
No. of Printed Pages : 7 BAS01.0 B.TECH. (AEROSPACE ENGINEERING) PROGRAMME (BTAE) CV CA CV C:) O TermEnd Examination December, 2011 BAS010 : MACHINE DESIGN Time : 3 hours Maximum Marks : 70 Note : (1)
More informationPENETRATION AND INDENTATION ON BASALT FIBRE REINFORCED PLASTIC LAMINATES UNDER LOW VELOCITY IMPACTS
PENETRATION AND INDENTATION ON BASALT FIBRE REINFORCED PLASTIC LAMINATES UNDER LOW VELOCITY IMPACTS V. Lopresto*, G. Caprino, A. Langella, C. Leone Department of Materials and Production Engineering, University
More informationCOMPOSITE MATERIALS. Asst. Prof. Dr. Ayşe KALEMTAŞ
COMPOSITE MATERIALS Office Hours: Tuesday, 16:3017:30 akalemtas@mu.edu.tr, akalemtas@gmail.com Phone: +90 252 211 19 17 Metallurgical and Materials Engineering Department CONTENT Composite Materials Metal
More informationDETERMINATION OF TIMETEMPERATURE SHIFT FACTOR FOR LONGTERM LIFE PREDICTION OF POLYMER COMPOSITES
DETERMINATION OF TIMETEMPERATURE SHIFT FACTOR FOR LONGTERM LIFE PREDICTION OF POLYMER COMPOSITES K. Fukushima*, H. Cai**, M. Nakada*** and Y. Miyano*** * Graduate School, Kanazawa Institute of Technology
More informationDeflection Calculation of RC Beams: Finite Element Software Versus Design Code Methods
Deflection Calculation of RC Beams: Finite Element Software Versus Design Code Methods G. Kaklauskas, Vilnius Gediminas Technical University, 1223 Vilnius, Lithuania (gintaris.kaklauskas@st.vtu.lt) V.
More informationMECHANICS OF MATERIALS
T dition CHTR MCHNICS OF MTRIS Ferdinand. Beer. Russell Johnston, Jr. John T. DeWolf ecture Notes: J. Walt Oler Texas Tech University Stress and Strain xial oading  Contents Stress & Strain: xial oading
More informationQUALIFICATION OF MATERIALS AND BLADES FOR WIND TURBINES. Jakob WedelHeinen and Josef Kryger Tadich
Proceedings of the 27 th Risø International Symposium on Materials Science: Polymer Composite Materials for Wind Power Turbines Editors: H. Lilholt, B. Madsen, T.L. Andersen, L.P. Mikkelsen, A. Thygesen
More informationProductprocess interaction modeling of composite structures using AsBuilt information
FASERINSTITUT BREMEN e.v. (FIBRE) Productprocess interaction modeling of composite structures using AsBuilt information Christian BRAUNER 1, Andrea MIENE 1, Michael BRUYNEEL², Frederic PASCON², Axel
More informationOn certification aspects of wind turbine blade load carrying structure
On certification aspects of wind turbine blade load carrying structure Tomasz Sieradzan, Bente Vestergaard Lead author: Tomasz.sieradzan@dnvgl.com Direct: +45 3945 4879 DNV GL Tuborg Parkvej 8, 2 nd floor
More informationSelecting materials at an early product design stage tools and methods
ENGINEERING DESIGN Selecting materials at an early product ROUNDTABLES March 17, 2015 Selecting materials at an early product design stage tools and methods Arlindo Silva et al. Instituto Superior Tecnico
More informationThermoplastic composites
Thermoplastic composites Definition By definition, a thermoplastic is a material based on polymer (macromolecular compound) which can be shaped, in a liquid (viscous) state at a temperature either higher
More informationMultiaxial Fatigue. Professor Darrell Socie. 20082014 Darrell Socie, All Rights Reserved
Multiaxial Fatigue Professor Darrell Socie 20082014 Darrell Socie, All Rights Reserved Outline Stresses around holes Crack Nucleation Crack Growth MultiaxialFatigue 20082014 Darrell Socie, All Rights
More informationComparative Cost Study of a 35m Wind Turbine Blade using Infusion and Prepreg Materials Technology
Comparative Cost Study of a 35m Wind Turbine Blade using Infusion and Prepreg Materials Technology Introduction Wind turbine blades are manufactured using advanced composite materials due to their specific
More informationUSE OF CFRP LAMINATES FOR STRENGTHENING OF REINFORCED CONCRETE CORBELS
International Journal of Civil Engineering and Technology (IJCIET) Volume 6, Issue 11, Nov 2015, pp. 1120, Article ID: IJCIET_06_11_002 Available online at http://www.iaeme.com/ijciet/issues.asp?jtype=ijciet&vtype=6&itype=11
More informationFinite Element Formulation for Beams  Handout 2 
Finite Element Formulation for Beams  Handout 2  Dr Fehmi Cirak (fc286@) Completed Version Review of EulerBernoulli Beam Physical beam model midline Beam domain in threedimensions Midline, also called
More informationCarbon Fiber Reinforced Polymer (CFRP) Laminates  Aslan
Carbon Fiber Reinforced Polymer (CFRP) Laminates  Aslan 400 series November 10, 2011 Aslan 400 Carbon FRP Laminates are used to structurally strengthen existing concrete, wood, or masonry members in flexure
More informationThree dimensional thermoset composite curing simulations involving heat conduction, cure kinetics, and viscoelastic stress strain response
Three dimensional thermoset composite curing simulations involving heat conduction, cure kinetics, and viscoelastic stress strain response Harrison Poon, Seid Koric, M. Fouad Ahmad National Center for
More informationDesign and Analysis of a Storage Container Used in Missile
Design and of a Storage Container Used in Missile 75 Prudvi Raju. Devarapalli M.Tech Student Technology, Ongole Venkata Ramesh Mamilla Associate Professor Technology Ongole M.V. Mallikarjun Professor Technology
More informationAdam Zaborski handouts for Afghans
Tensile test Adam Zaborski handouts for Afghans Outline Tensile test purpose Universal testing machines and test specimens Stressstrain diagram Mild steel : proportional stage, elastic limit, yielding
More informationEFFECT OF CURE CYCLE ON THE PROPERTIES OF THICK CARBON/EPOXY LAMINATES
EFFECT OF CURE CYCLE ON THE PROPERTIES OF THICK CARBON/EPOXY LAMINATES M. R.L. Gower, R. M. Shaw and W.R. Broughton National Physical Laboratory Hampton Road, Teddington, Middlesex, TW11 LW, United Kingdom
More informationMicroscopy and Nanoindentation. Combining Orientation Imaging. to investigate localized. deformation behaviour. Felix Reinauer
Combining Orientation Imaging Microscopy and Nanoindentation to investigate localized deformation behaviour Felix Reinauer René de Kloe Matt Nowell Introduction Anisotropy in crystalline materials Presentation
More informationMohr s Circle. Academic Resource Center
Mohr s Circle Academic Resource Center Introduction The transformation equations for plane stress can be represented in graphical form by a plot known as Mohr s Circle. This graphical representation is
More informationMASTER DEGREE PROJECT
MASTER DEGREE PROJECT Finite Element Analysis of a Washing Machine Cylinder Thesis in Applied Mechanics one year Master Degree Program Performed : Spring term, 2010 Level Author Supervisor s Examiner :
More informationQuestion 2: How do you solve a matrix equation using the matrix inverse?
Question : How do you solve a matrix equation using the matrix inverse? In the previous question, we wrote systems of equations as a matrix equation AX B. In this format, the matrix A contains the coefficients
More informationČeské vysoké učení technické v Praze Fakulta strojní DIPLOMOVÁ PRÁCE. Analysis of the Composite Beam Bending. Analýza ohybu kompozitních nosníků
České vysoké učení technické v Praze Fakulta strojní DIPLOMOVÁ PRÁCE Analysis of the Composite Beam Bending Analýza ohybu kompozitních nosníků 2015 Tereza ZAVŘELOVÁ Anotační list Jméno autora: Tereza ZAVŘELOVÁ
More informationXantu.LayrTM nanofibre interleaving veils provide a technological leap forward for the toughening of high performance composites.
Continuous Nanofibre. Performance composites Xantu.LayrTM nanofibre interleaving veils provide a technological leap forward for the toughening of high performance composites. Xantu.LayrTM enhances composite
More informationComposite structures are used extensively in aircraft, space vehicles, marine, and automotive
Finite Element Analyses of CompositetoSteel Adhesive Joints YuPing Yang George W. Ritter David R. Speth Edision Welding Institute Columbus, Ohio Finite element modeling can assist in the design of an
More informationMATERIALS AND MECHANICS OF BENDING
HAPTER Reinforced oncrete Design Fifth Edition MATERIALS AND MEHANIS OF BENDING A. J. lark School of Engineering Department of ivil and Environmental Engineering Part I oncrete Design and Analysis b FALL
More informationNAVAL POSTGRADUATE SCHOOL Monterey, California THESIS
NAVAL POSTGRADUATE SCHOOL Monterey, California THESIS MULTILEVEL TECHNIQUE FOR STIFFNESS AND STRENGTH CALCULATIONS OF WOVEN FABRIC COMPOSITE PLATE AND SHELL STRUCTURES by Ahmet Altekin June 2001 Thesis
More informationHighTech Plastics for Lightweight Solutions
HighTech Plastics for Lightweight Solutions Julian Haspel, High Performance Materials, Global Application Development Mobility Days Prague, November 22nd 2012 Agenda Plastic / metal hybrid technology
More informationCarbon Fiber Reinforced Polymer (CFRP) as Reinforcement for Concrete Beam
Carbon Fiber Reinforced Polymer (CFRP) as Reinforcement for Concrete Beam Norazman Mohamad Nor 1, Mohd Hanif Ahmad Boestamam, Mohammed Alias Yusof 3 1,3 Universiti Pertahanan Nasional Malaysia, 57000 Kuala
More informationAPE T CFRP Aslan 500
Carbon Fiber Reinforced Polymer (CFRP) Tape is used for structural strengthening of concrete, masonry or timber elements using the technique known as Near Surface Mount or NSM strengthening. Use of CFRP
More informationNonlinear analysis and formfinding in GSA Training Course
Nonlinear analysis and formfinding in GSA Training Course Nonlinear analysis and formfinding in GSA 1 of 47 Oasys Ltd Nonlinear analysis and formfinding in GSA 2 of 47 Using the GSA GsRelax Solver
More informationTIE31: Mechanical and thermal properties of optical glass
PAGE 1/10 1 Density The density of optical glass varies from 239 for NBK10 to 603 for SF66 In most cases glasses with higher densities also have higher refractive indices (eg SF type glasses) The density
More informationGrade 6 GradeLevel Goals. Equivalent names for fractions, decimals, and percents. Comparing and ordering numbers
Content Strand: Number and Numeration Understand the Meanings, Uses, and Representations of Numbers Understand Equivalent Names for Numbers Understand Common Numerical Relations Place value and notation
More information